```MME 467: Ceramics for Advanced Applications
Lecture 23
Superconductivity
Ref: Richerson, Dekker, 2nd Ed., 1992, pp.239–248.
Prof. A. K. M. B. Rashid
Department of MME, BUET, Dhaka
Topics to discuss .......
!
q  Discovery and development!
q  Properties and theory!
q  Applications!
1 What is a Superconductor ?
q  Superconductivity is the ability of certain materials to conduct
electrical current with no resistance.
q  Thus, superconductors can carry large amounts of current with
little or no loss of energy.
q  Most materials will only superconduct, at very low temperatures,
near absolute zero.
q  Above a certain critical temperature, Tc, the material may have
conventional metallic conductivity or may even be an insulator.
q  As the temperature drops below the critical point, resistivity rapidly
drops to zero and current can flow freely without any resistance.
Linear reduction in resistivity as temperature is decreased:
ρ = ρ0 "#1+ α (T −T0 )\$%
ρ = resistivity
α = the linear temperature coefficient of resistivity.
Resistivity: ρs ~ 4x10-23 Ω cm for superconductor.
Resistivity: ρm ~ 1x10-13 Ω cm for non-superconductor metal.
2 Superconductors have two outstanding features:
[1] Zero electrical resistivity
q  This means that an electrical current in a superconducting ring
continues indefinitely until a force is applied to oppose the current.
[2] The magnetic field inside a bulk sample is zero
(the Meissner effect)
q  When a magnetic field is applied, current flows in the outer skin
of the material leading to an induced magnetic field that exactly
opposes the applied field.
q  The material becomes strongly diamagnetic as a result.
q  In the Meissner effect experiment, a magnet floats above the
surface of the superconductor.
Discovery & Development
Heike Kammerlingh Onnes
(1853 – 1926)
1908:
Liquid He with a boiling temperature of 4.2 K
1911:
Mercury with liquid He cooling
è No resistance measured (<10-27Ω⋅m)
“When the temperature cooled to ~4.2 K,
mercury has passed to a new state, may be
called the superconductive state”
The Kamerlingh Onnes resistance
measurement of mercury.
Noble Prize on low temperature
physics in 1913
At 4.15K, the resistance suddenly
dropped to zero.
3 q  Sn: ~3.8 K; Pb: ~6 K
q  Current was running after one year in a loop of Pb wire
cooled in liquid He.
q  V & Nb were also found to be superconducting with low
superconducting temperatures and current densities. Once a
current exceeds the critical current density, or if there is a
magnetic field which exceeds the critical field, the material
becomes non-superconducting.
Alloys and metallic compounds
(from 1950)
u  V3Si
u  Nb3Sn
u  Nb3Ge
: 17 K (1952)
: 18 K
: 23 K (1973)
q  Have much higher critical temperature (Tc), current density (Jc) and
critical magnetic field (Hc)
è Essential for providing high magnetic fields.
q  Nb3Ti & Nb3Sn : Jc = ~106A/cm2
è Superconducting magnets for magnetic resonance imager (MRI)
& scientific research.
Other chemical compounds:
u  NbN
: 17.3 K
u  PbMo6S7
: 15.2 K
u  MoC
: 14.3 K
4 High temperature superconductors
La-Ba-Cu-O system:
q  Bednorz and Müller in IBM Zurich in January 1986; Tc ~30 K
q  Further confirmed by the researchers from Tokyo University on the
Fall Meeting of Materials Research Society (MRS) in Boston.
The discovery of
superconductivity in
ceramic materials
The Nobel Prize
in Physics in 1987
K. A. Muller
J. G. Bednorz
Y-Ba-Cu-O system (YBCO)
YBa2Cu3O7-d
Y123
Tc = ~92 K
Has two crystal structures:
i)
d< 0.5, orthorhombic; a= 3.827, b= 3.882, and c= 11.682 Å;
this phase is superconductive;
ii) d> 0.5, tetragonal; a= b= 3.9018, and c= 11.9403 Å;
this phase is non-superconductive
Tc is a function of oxygen contents, an oxygen annealing is needed to
ensure high oxygen contents in order to achieve the highest possible Tc;
The lower critical field Hc1 is low, but Hc2 is high, ~200-300 Tesla at 0 K;
Single crystal : Jc = 1.5x106A/cm2 at 4 K, 1x104A/cm2 at 77 K
Polycrystalline : 100-1000 A/cm2 at 77 K
Film
: 5x107 A/cm2 at 4 K at 0-1 T field, 5x106A/cm2 at 77 K
YBa2Cu4O8
Y2Ba4Cu7O14
Y124
Y247
Tc = ~85 K
Tc = ~92 K
5 Bi-Sr-Ca-Cu-O system: 1988 by H. Meada (Japan)
Bi2Sr2CuO6
Bi2Sr2CaCuO7
Bi2Sr2Ca2Cu3O10
Bi2201
Bi2212
Bi2223
Tc< 30 K
Tc= ~85 K
Tc=110 K
q  Bi2212 & Bi2223 have perovskite structure with tetragonal unit cells;
Bi2212 has 2 layers of Cu-O and Bi2223 has 3 layers of Cu-O
q  Comparison between YBCO and BSCCO:
i)
Bi2223 has a higher Tc than YBCO;
ii)
BSCCO crystals cleave easily along (001) planes, making it easy
to be textured with mechanical deformation;
iii) No “oxygenation” process is needed because the oxygen content
in BSCCO is relatively stable
iv)
BSCCO compounds have better stabilities in water containing
environments
Tl-Ba-Ca-Cu-O system
By Shen & Hermann with Tc = ~125 K;
q
q
q
q
Have a higher Tc than YBCO and BSCCO superconductors;
Their crystal structures are similar with tetragonal unit cells;
Jc and Hc are also high
Highly poisonous
Hg-Ba-Cu-O system
Hg-Ba-Ca-Cu-O system
By Houston University with Tc = ~130-160 K
q  Superconductors with Tc around 200 K, 250 K, and even 0ºC were
reported but were too difficult to reproduce.
HTSC thin films:
YBCO thin films by sputtering, laser deposition, molecular beam
epitaxy, and metal-organic chemical vapour deposition
6 Properties & Theory
1. Critical temperature (Tc)
q  The critical transition temperature
below which a normal conducting
material loses its resistivity and
begins to be superconductive.
ρ
Pure
metals
q  Tc is definite for a material.
Alloys and
ceramics
q  The superconducting transition is
reversible !!
q  The transition temperature often
varies with the atomic mass, ma,
according to
(ma)α TC = Constant
1–2K
TC
T α = material constant (isotope effect)
As an example, TC for mercury varies from 4.185 K to 4.146 K
when ma changes from 199.5 to 203.4 atomic units.
7 Critical Temperatures of Some Superconducting Materials
Materials
TC (K)
Materials
Elements
Tungsten
Titanium
Zirconium
Zinc
Uranium
Aluminium
Tellurium
Mercury
Niobium
0.01
0.53
0.70
0.79
0.80
1.14
2.38
4.15
7.26
9.22
Compounds
PbTl2
V3Si
Nb3Sn
Nb3Ge
Ceramic compounds
La2Ba2CuO4
YBa2Cu3O7
Bi2Sr2Ca2Cu3O10
Tl2Ba2Ca2Cu3O10
HgBa2Ca2Cu2O8
TC (K)
3.8
17.1
18.3
23.0
40.0
92.0
110.0
125.0
133.0
q  Depending on Tc, two types of superconductor:
[1] Low Tc superconductors
[2] High Tc superconductors
Effect of Variables on Tc
Effect of Pressure
Pressure ↑, TC ↑
High TC superconductors – High pressure
Thermal Properties
Entropy & Specific heat ↓ at TC
Disappearance of thermo electric effect at TC
Thermal conductivity ↓ at TC – Type I superconductors
Stress
Stress ↑, dimension ↑, TC ↑, HC affected
Frequency
Frequency ↑, Zero resistance – modified, TC not affected
8 2. Critical magnetic field
q  The “critical field” or maximum magnetic field that a superconductor
can endure before it is “quenched” and returns to a non-superconducting
state.
q  Usually a higher Tc also brings a higher Hc.
Type-I superconductor: metals
(exclusive V & Nb)
Type-II superconductor: V, Nb, alloys,
compounds and HT SC
!
T =0 K
T =Tc
0 <T <Tc
dH c
=0
dT
Hc = 0
dH c
<0
dT
( " %2 +
T
H c (T ) = H c (0) *1− \$ ' * #Tc & )
,
Critical field at T = 0 K
9 The critical magnetic flux density (BC) and magnetic field
at 0 K (H0) of a number of superconducting materials
Materials
BC (telsa)
H0 (A/m)
Materials
Tungsten
Titanium
Aluminium
Tin
Mercury
Niobium
0.0001
0.0056
0.0105
0.0305
0.0411
0.0803
91.5
4450-7960
8360
24300
32700
63900
156800
Nb-Ti alloy
Nb-Zr alloy
Pb8Mo6S8
V3Ga
Nb3Sn
Nb3Al
Nb3Ge
BC (telsa)
12
11
45
22
22
32
30
q  On the basis of magnetic response, superconducting materials may
be divided into two classifications designated as type I and type II.
ρ
Type I
Superconductor
ρ
Type II
Superconductor
HC1
HC
H
v  Sudden loss of magnetisation
v  Exhibit Meissner Effect
v  No mixed state
v  Hc ~ 1 tesla
v  Soft superconductor
v  Eg. – Al, Pb, Sn, Hg
HC2
H
v  Does not exhibit complete Meissner Effect
v  Two HCs – HC1 & HC2 (≈30 tesla)
v  Mixed state present
v  Hard superconductor
v  Eg. – Nb-Sn, Nb-Ti, ceramic SCs
10 3. Critical current
q  The magnetic field that causes a superconductor to become normal
is not necessarily an external applied field; it may also arise as a
result of electric current flow in the conductor.
q  superconductivity in a long circular wire of radius r may be
destroyed when the current I exceeds the value IC, which at the
surface of the wire produce the critical magnetic field HC.
Hence, the critical current
I c = 2π rH c
Silsbee’s rule !
The superconducting envelope, showing the combined effects of temperature, magnetic
field, and current density. Conditions within the envelope produce superconductivity.
11 4. Meissner effect
a) When a magnetic field is applied to a
conducting material, the changing
flux creates an electric field that sets
up eddy current, which opposes the
applied magnetic field.
Diamagnetism tied to zero electrical
resistance (i.e., ρ = 0 and B = 0) in a
superconducting material results in special
behaviour referred to as the Meissner effect.
b) Because of the resistivity of material,
eddy current decays, and the lines of
magnetic force penetrate the material
as if it were not there.
!
c) In case of superconductor, because of
the absence of resistivity, eddy
currents do not decay. They produce
a mirror image magnetic field that
completely cancels the applied
magnetic field.
Representation of the Meissner effect. (a) While in
superconducting state, a body of material (circle)
excludes a magnetic field (arrow) from its interior. (b)
The magnetic field penetrates the same body once it
becomes normally conductive.
!
Thus, a semiconductor may be
regarded as a perfect diamagnet,
where the magnetic field does not
penetrate, but is repelled.
Magnetic Levitation
q  Magnetic fields are actively excluded
from superconductors (Meissner effect).
q  If a small magnet is brought near a
superconductor, it will be repelled
because the induced supercurrents will
produce mirror images of each pole.
q  If a small permanent magnet is placed
above a superconductor, it can be
levitated by this repulsive force
q  The Meissner effect is limited by the strength of the flux.
q  Strong fields will destroy superconductivity and the Meissner effect
will disappear.
12 BCS Theory of Superconductivity
q  A pair of electrons close to the
Fermi level will couple into a
Cooper pair through interaction
with the crystal lattice.
q  This pairing results from a slight
attraction between the electrons
related to lattice vibrations.
1
q  The motions of all of the Cooper pairs
within a single superconductor are
correlated; they constitute a system that
functions as a single entity.
2
Phonon
Schematic of a Cooper pair
q  Application of an electrical voltage to the
superconductor causes all Cooper pairs
to move, constituting a current.
q  When the voltage is removed, current
continues to flow indefinitely because the
pairs encounter no opposition.
q  For the current to stop, all of the Cooper
pairs would have to be halted at the same
time, a very unlikely occurrence.
!
Schematic illustration of the BCS theory illustrating the difference
between normal conduction and zero-resistance superconduction
q  A finite amount of energy is needed to break Cooper pair apart into two
independent electrons. This means there is an “energy gap” for “single-particle
excitation”.
q  As temperature increases, more electron pairs will be broken up, and the
attractive force in the unbroken pairs will be decreased.
q  At a critical temperature, all the electron pairs will be broken, the energy gap
vanishes and superconductivity ceases to exist. This temperature is the critical
transition temperature of superconductivity.
13 Applications
1) Superconductor magnets:
q  A small magnet can provide a huge magnetic field; the energy loss
is minimum
q  Current & potential industrial applications: Magnetic resonance
imaging system (MRI) for medical diagnostics and research; Ore
Magnetic shielding
2) Electric power utilities:
q  Power transmission; Superconducting generators & motors;
Superconducting magnetic energy storage (SMES); Transportation
tools; Josephson effect; Superconducting quantum interface
devices (SQUID)
Cost Saving
Zero resistance,
no energy lost,
novel uses…
and
Cost Increase
Need refrigeration,
fabrication costs….
14 Superconducting Cable
q  The cable configuration features a
wound around a flexible hollow core.
q  Liquid nitrogen flows through the core,
cooling the HTS wire to the zero
resistance state.
q  The conductor is surrounded by
conventional dielectric insulation. The
efficiency of this design reduces losses
Magnetic Levitated Train
q  1960s, Dr. H. Kolmat MIT suggested that a train would fly along a
frictionless track supported by a powerful magnetic field
è magnetically levitated train
q  1987, the Japanese demonstrated a prototype maglev train, MLU-002,
travelled520km/hour and flied ~10 cm above the track
Principle:
Electro-magnetic induction
Magnetic levitation transport, or maglev, is a
form of transportation that suspends, guides and
propels vehicles via electromagnetic force. This
method can be faster than wheeled mass transit
systems, potentially reaching velocities comparable
to turboprop and jet aircraft (500 to 580 km/h).
15 v The track are walls with a continuous series of vertical coils of wire
mounted inside. The wire in these coils is not a superconductor.
v As the train passes each coil, the motion of the superconducting
magnet on the train induces a current in these coils, making them
electromagnets.
v The electromagnets on the train and outside produce forces that
levitate the train and keep it centered above the track. In addition, a
wave of electric current sweeps down these outside coils and propels
the train forward
q  No need of initial energy in case of magnets for low speeds
q  One litre of liquid nitrogen costs less than one litre of mineral water
q  Onboard magnets and large margin between rail and train enable
highest recorded train speeds (581 km/h) and heavy load capacity.
Successful operations using high temperature superconductors in its
onboard magnets, cooled with inexpensive liquid nitrogen
q  Magnetic fields inside and outside the vehicle are insignificant;
proven, commercially available technology that can attain very high
speeds (500 km/h); no wheels or secondary propulsion system needed
q  Free of friction as it is “Levitating”
16 Medical Applications
q  MRI (Magnetic Resonance Imaging) scans produce detailed
images of soft tissues.
q  The superconducting magnet coils produce a large and uniform
magnetic field inside the patient's body.
Next Class
Lecture 27
Magnetic Properties
17 ```